Loading in 2 Seconds...
Loading in 2 Seconds...
Navy Qualification Effort for HVOF Wear-Resistant Actuator Rod Coatings. Project Status as of 1 April 2003. Project History. History of leakage related premature actuator removals prompted work in this area. Initial efforts evaluated high temperature elastomer seals.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Project Status as of 1 April 2003
History of leakage related premature actuator removals prompted work in this area.
Initial efforts evaluated high temperature elastomer seals.
Lab endurance testing showed performance of PTFE spring energized seals far superior to elastomer seals.
Laboratory testing showed super-finished HVOF coated rods have superior wear resistance compared to chrome plated rods.
Although existing aircraft hydraulic systems are rated for 275ºF, Buna-N seals are damaged above 160ºF.
In 1996, several actuators were repacked with high temperature fluorocarbon rated for 350ºF.
Actuators were tested at elevated temperatures and static seals showed excellent performance, but seals were damaged in a couple dynamic applications.
Canadian forces have flown a fluorocarbon equipped F/A-18 test aircraft since 1997 with no measurable leakage.
In 2000, several seal configurations were compared in high and low temperature endurance testing (baseline Buna-N, improved nitrile, hydrogenated nitrile, fluorocarbon, fluorosilicon and spring energized PTFE seals).
Although better than Buna-N, all engineered elastomer seals eventually showed degradation and leakage, some leaving tar-like debris (internal and external).
Spring energized PTFE seals showed superior performance and many had no measurable leakage.
6 layers of testing, 16 hours each layer.
Each hour consists of 20 minutes full stroke, 20 minutes of superimposed dither and 20 minutes of dither stroke.
First layer is 160ºF, second layer is 300ºF, third layer is 275ºF and temperature is reduced 25ºF each subsequent layer.
Seal blocks are chilled to 0ºF each night to evaluate static leakage.
After layer 6, stand is cold soaked to –40ºF and 4 hours of additional testing is performed to evaluate extreme low temperature and cumulative seal damage.
Total Time: 100 Hours
Full Stroke Testing-
3 ½ Inch Stroke
1 ½ Second Period
Dither in place –
¼ Inch Stroke
2 seals leaked early on and continued steady leakage suggesting a design problem.
While excellent at high and low temperatures Fluorosilicon is easily damaged in a dynamic environment (not acceptable).
Nitrile and Improved Nitrile baseline seals have proven unacceptable in this test and in the field.
Engineered elastomers of Viton, HNBR all showed steady leakage with increased leakage during low temperature startup. Elastomer degradation also produced a tar like sludge at the rod seal interface.
Several PTFE spring energized seals showed no measurable leakage through testing.
Once PTFE spring energized seals were selected, 4 different rod configurations were tested against the PTFE seals.
Coated Rod configuration:
Rod #1 - WC/17Co
Rod #2 - WC/10Co4Cr
Rod #3 - WC/17Co (0.010” Thickness)
Rod #4 - Tribaloy 400
Chrome plated rods under these conditions developed longitudinal scratches, which is also a common problem on chrome plated rods on aircraft actuators.
Inspection of HVOF rods showed wear marks and polishing but the accumulated surface damage was much less severe than with chrome plated test rods.
Initial surface finish is critical because wear resistant HVOF rods will not polish up in service.
Axial scratching and galling after 100 hour endurance test
After 100 hour endurance test, no visible surface damage
History of significant reliability problems due to external leakage with actuators reworked every 6 months.
Based on laboratory results, fluorocarbon was selected for static seals and PTFE spring energized dynamic seals were selected for dynamic applications.
Rebuild kits for F/A-18 C/D stabilator actuator were developed by seal vendors using hardware dimensions.
Endurance testing of seal kits from three vendors showed excellent performance and post-test leakage within ATP limits.
Actuator reworked with AMS-R-83485 fluorocarbon static seals and PTFE dynamic seals tested to the following spectrum.
10 layers of testing.
Each hour consists of 3 minutes full stroke, 9 minutes of half stroke and 48 minutes of dither stroke
One layer at 275ºF, two layers at 250ºF, three layers at 225ºF and four layers at 185ºF.
Actuator was chilled to -40ºF each night to evaluate static leakage.
All vendors tested seals acceptable with no external leakage and acceptable internal leakage after endurance testing.
Follow-on testing evaluated HVOF coated rod against these seals.
Leakage performance was equivalent to chrome plated rod.
This actuator will be flown on a test aircraft to evaluate in-service wear and corrosion resistance.
History of significant leakage problems with actuators replaced every 6 months.
Fluorocarbon selected for static seals and PTFE spring energized dynamic seals selected for dynamic rod seals.
Side by side design allows one chrome rod and one HVOF rod to evaluate seals against both rod surfaces.
Endurance testing of first modified TEF actuator should begin next week.
Pending successful lab testing, these modified actuators will be flown to evaluate in-service corrosion and wear resistance.
4 actuators with HVOF coated rods in service for ~2 years.
Actuators have accumulated 704 flight hours.
Visual inspection shows no corrosion or external leakage.
Program is working to approve HVOF as an alternate repair procedure.
Endurance and flight testing of fluorocarbon seals and PTFE spring energized dynamic seals for TEF actuators on HVOF coated and chrome plated piston rods.
Authorize HVOF for repair of actuator rods and develop HVOF production capability for Navy Repair Depots.
Pending successful testing, extend HVOF repair to similar applications on other hydraulic actuator and damper rods.
Investigate repair techniques for damaged internal surfaces.